Amino Acids in Iron Oxide Mineralization: (Incomplete) Crystal Phase Selection Is Achieved Even with Single Amino Acids
Alexandre Mantion,†,OFabia Gozzo,‡Bernd Schmitt,‡Willem B. Stern,§Yvonne Gerber,§ Adeline Y. Robin,|Katharina M. Fromm,⊥Monika Painsi,#and Andreas Taubert*,†,3 Department of Chemistry, UniVersity of Basel, CH-4056 Basel, Switzerland, Swiss Light Source,
Paul-Scherrer-Institute, CH-5232 Villigen, Switzerland, Department of EnVironmental Geosciences, UniVersity of Basel, CH-4056 Basel, Switzerland, Laboratoire de cristalloge´ne`se et cristallographie des prote´ines, Institut de Biologie Structurale Jean-Pierre Ebel, CEA-CNRS-UniVersity J. Fourier, F-38027 Grenoble, France, Department of Chemistry, UniVersity of Fribourg, CH-1700 Fribourg, Switzerland, Institute of Geological Sciences, UniVersity of Bern, CH-3012 Berne, Switzerland, Institute of Chemistry, UniVersity of Potsdam, D-14476 Golm, Germany, and Max-Planck-Institute of Colloids and Interfaces, D-14476, Golm, Germany
Iron oxides are important minerals in biology and materials science. Using biomimetic synthesis, a variety of iron oxides have been fabricated. However, it is still not clear how growth modiﬁers like amino acids and peptides select different crystal phases of a complex material like iron oxide. The current paper shows that already with single amino acids, (incomplete) crystal phase selection is achieved in vitro. In particular,
L-histidine, L-threonine, and L-cysteine favor the formation of unstable crystal phases like ferrihydrite or lepidocrocite, although sometimes only at high amino acid concentrations. Other amino acids like L-valine have only minor effects when compared to control samples grown in the absence of amino acids. The effects of the amino acids can be rationalized via kinetic trapping and different interaction strengths of the amino acids with the growing iron oxide particles. The effects of the amino acids on the particle morphologies are less signiﬁcant. The paper therefore shows that single amino acids can be a valuable tool for the materials chemist to fabricate and stabilize even unstable iron oxide crystal phases.
Iron oxides and hydroxides are among the most important minerals in biology and technology.1–4Biomimetic iron oxide particles have been made from a range of iron salts, and a wide variety of particles, including functionalized particles for nanomedicine, has been obtained.4–8 Despite the successful implementation in several branches of technology, the details of iron oxide mineralization both in vivo and in vitro are a subject of ongoing research.9–22For example, Mann et al. have studied the formation of iron oxides and oxyhydroxides using phospholipid vesicles as a model system.9 Banﬁeld and co- workers have studied the mineralization of iron oxides on a polymer-based scaffold and have suggested reasons why some microbes release polysaccharide-templated iron oxohydroxides.15,16 The thermochemistry of iron oxides and oxyhydroxides is also still under investigation,12,23 in particular interconversion processes.13,14,17–19
There is little knowledge on how peptides and other biological or organic molecules control iron oxide mineralization. How- ever, there are some data on the interaction of organic molecules
with preformed iron oxide particles. Brown has shown that proteins containing a basic oligopeptide, Arg-Arg-Val-Thr-Lys- His-His-Val-Asn, adsorb on Fe2O3but not on Fe3O4.24,25Arakaki et al. have found an acidic protein tightly bound to magnetite, Fe3O4.26 Prozorov et al. have shown that the same protein induces the formation of magnetic nanoparticles.27Matrajt and Blanot have shown that different amino acids interact differently with ferrihydrite.28Similar interactions exist for other inorganic/
peptide combinations,29but even the mineralization of a simple compound like ZnO is more complex with peptides30,31 than with synthetic polymers.32–34 As a result, there is a need to further study the role of biomimetic additives on the mineraliza- tion of iron oxides.
The current work is inspired by the work of Brown, who has shown that the oligopeptide Arg-Arg-Val-Thr-Lys-His-His-Val- Asn adsorbs on Fe2O3but not on Fe3O4.24In order to determine if there is already an effect of the individual components of this oligopeptide (that is, the single amino acids), we have precipitated iron oxide in the presence of different concentrations of these amino acids. For comparison, we have also included the sulfur-containing amino acidsL-cysteine andL-methionine, which are known to strongly coordinate to iron.35 The paper clearly shows that already single amino acids have a strong inﬂuence on iron oxide crystal phase selection from aqueous solution, although there is no complete suppression of other crystal phases.
Preparation of Iron Oxides.Chemicals were obtained from Fluka and used as received. For precipitation, 50 mL of an aqueous amino acid solution and 20 mL of an aqueous 80 mM
* Corresponding author. Phone:++49 (0)331 977 5773. E-mail: ataubert@
†Department of Chemistry, University of Basel.
§Department of Environmental Geosciences, University of Basel.
|CEA-CNRS-University J. Fourier.
⊥University of Fribourg.
#University of Bern.
3University of Potsdam and Max-Planck-Institute of Colloids and Interfaces.
OCurrent address: Department of Chemistry, Humboldt University, Brook-Taylor-Str. 2, D-12489 Berlin, Germany.
Published in "The Journal of Physical Chemistry C 112(32): 12104–12110, 2008"
which should be cited to refer to this work.
FeSO4(NH4)2SO4·6H2O solution were mixed under stirring.
Then 10 mL of a 12 M aqueous ammonia solution were added under stirring. Amino acid concentrations were set such that the ﬁnal concentration after mixing these solutions was 0.1, 1, 10, or 100 mM. In the case of histidine and threonine, the maximum concentrations were 60 and 80 mM, respectively, due to their limited solubility. During the whole process, air was bubbled through the reaction solution with an aquarium pump at 10 L/hr. During reaction, the pH remained at pH 9. After 24 h, the suspensions were centrifuged, the supernatant was decanted, and the solids were air-dried at 40°C.
Characterization.XRD was done at the Swiss Light Source, Paul-Scherrer-Institute, Beamline X04SA. Patterns were re- corded from 1° to 60° 2θ using the MYTHEN microstrip detector.36 Samples were mounted in 1 mm mark tubes (Hilgendorf) and measured while rotating. X-ray wavelengthλ was 0.708 Å and electron energy was 17.5 keV. Peaks were modeled using a Pseudo Voigt model (Thompson-Cox-Hastings pseudo-Voigt convoluted with Axial divergence asymmetry) using Fullprof.37Atomic positions were used as published.3For TEM, particles were dispersed in ethanol and deposited on carbon coated copper grids. Samples were imaged with a Philips Morgagni TEM at 80 kV. TGA was done on a Mettler Toledo TGA/SDTA851e from 25 to 600°C with heating rates of 10-40
°C/min under nitrogen (10 mL/min) in alumina crucibles. IR spectra were recorded on a Shimadzu FTIR 8300 with a Golden Gate ATR probe from 650 to 4000 cm-1. Raman microscopy was done with an Olympus BX 41 (100 x objective) optical microscope coupled to a Labram HR800 Jobin Yvon Horiba Raman spectrometer with a 514 nm laser with a power of 5.20 mW. XRF spectra were recorded on an energy-dispersive Spectro X-LABORATORY 2000 using the “police tape”
Crystal phases of the precipitates were determined via synchrotron powder X-ray diffraction (XRD). Rietveld reﬁne- ment was used to determine the relative amounts of individual crystal phases present in each sample. Figure 1 shows repre- sentative XRD patterns. Already visual inspection of the patterns shows that there are big differences between individual samples.
Some samples appear well crystallized, which is indicated by the rather narrow reﬂections, whereas others are so poorly crystalline that Rietveld reﬁnement was only possible with rather large errors or not possible at all.
Table 1 and Figure 2 summarize the results from XRD and Rietveld reﬁnement. Overall, the precipitates can be classiﬁed in two groups, which are plotted as the left and right column of Figure 2, respectively. Figure 2 shows that L-valine, L- methionine,L-asparagine, andL-arginine have a similar effect on mineralization. At low amino acid concentration, the sample is over 95% magnetite. Only withL-arginine, at 10 mM, a small fraction of goethite is found. At 100 mM of amino acid, other crystal phases are present in signiﬁcant amounts:L-valine and
L-methionine lead to mixtures of magnetite and lepidocrocite, whereas in the presence ofL-asparagine andL-arginine mixtures of magnetite, goethite, and lepidocrocite form. Furthermore, the weight fraction of magnetite decreases from L-valine to L- arginine and the fraction of goethite and the fraction of the less stable lepidocrocite increases.
The second group of precipitates does not exhibit as clear trends, but a few features can be found:L-lysine differs from the aforementioned samples in that already at 10 mM of amino acid, a signiﬁcant decrease in the magnetite content and corresponding increase in goethite content is found. At 100 mM, goethite is replaced by lepidocrocite and the magnetite fraction further decreases. At this point, it is interesting to compare the samples precipitated withL-asparagine,L-arginine, andL-lysine:
Figure 1. Representative X-ray patterns and Rietveld reﬁnement of samples precipitated in the presence of (a)L-valine (1 mM), (b)L-asparagine (80 mM), (c)L-arginine (10 mM), and (d)L-threonine (80 mM). The peak width affects the quality of the reﬁnement. The peaks in panel d are too broad for a successful reﬁnement. The residual curve is a measure of the quality of the ﬁt. For clarity reasons, the JCPDS peak positions of the respective iron oxides are not displayed. For crystal phases of the respective samples see Table 1.
these amino acids are more efﬁcient stabilizers for metastable crystal phases in increasing order.L-asparagine only leads to a
small fraction of goethite and lepidocrocite at high amino acid concentration. The fraction of these two crystal phases increases further withL-arginine and ﬁnallyL-lysine. Moreover,L-lysine has this effect at lower concentration.
L-Cysteine shows the same trend as L-lysine, but is more efﬁcient in that it already at low concentrations of 1 mM reduces the amount of magnetite to close to zero.L-Cysteine efﬁciently traps goethite and lepidocrocite at 1 mM and exclusively stabilizes lepidocrocite at 10 and 100 mM. Similar toL-cysteine,
L-threonine leads to goethite at 1 mM, lepidocrocite at 10 mM, and 2-line ferrihydrite at 100 mM.L-Histidine is exotic in that it does not appear to have an impact on the mineralization until at high concentrations of 100 mM. However, at this concentra- tion, the rather unstable ferrihydrite forms exclusively.
The above results clearly show that amino acids trap kinetically favored iron oxide crystal phases. The amino acids can be roughly arranged in order of increasing trapping efﬁciency. On this scale,L-valine is the least efﬁcient additive, followed by L-methionine, L-asparagine, L-arginine, L-lysine,
L-cysteine, and ﬁnally L-threonine. The latter two stabilize lepidocrocite and ferrihydrite, respectively, at high concentra- tions, but they also trap goethite and lepidocrocite at concentra- tions as low as 1 mM.
Figure 3 shows representative transmission electron micros- copy (TEM) images of some samples. Control samples and samples precipitated with 1 mM of amino acid (predominantly) contain rounded particles with a broad size distribution. At 10 and 100 mM, the morphologies vary. The particle morphologies are only poorly deﬁned and in many cases large aggregates are observed and the sizes of the individual particles vary signiﬁ- cantly within the sample as well as between the samples. This is in contrast to for example ZnO where both synthetic polymers and short peptides lead to well-deﬁned particles with a narrow size distribution.30–33,38,39TEM therefore shows that the amino acids used as growth modiﬁers are inefﬁcient in the sense that no uniform particle morphology and particle size is obtained.
TABLE 1: Iron Oxide Composition (wt %) as a Function of the Amino Acid (AA)a
amino acid 1 mM % 10 mM % 100 mMb %
L-valine magnetite 100 magnetite 100 magnetite 55
L-lysine magnetite 100 magnetite 65 magnetite 49
goethite 35 goethite 1
L-methionine magnetite 100 magnetite 98 magnetite 40
L-asparagine magnetite 97 magnetite 100 magnetite 29
goethite 3 goethite 17
L-arginine magnetite 100 magnetite 91 magnetite 2
goethite 9 goethite 31
L-histidine magnetite 100 magnetite 100 2-line ferrihydrite 100c
L-threonine magnetite 45 magnetite 24 2-line ferrihydrite 100c
goethite 55 goethite 27
L-cysteine magnetite 3
lepidocrocite 63 lepidocrocite 100 lepidocrocite/cystine hybridd N/a
aThe control sample is composed of 94% magnetite and 6% goethite. Representative X-ray patterns are given in Figure 1, crystallite sizes in Table 2, and stress-strain data are given in the Supporting Information, Table S2.bMaximum concentrations are 80 mM forL-threonine and 60 mM forL-histidine due to solubility limits.cThese reﬂections are too broad for Rietveld reﬁnement. Minor amounts of other crystal phases may have gone undetected.dSee discussion below.
Figure 2. Phase composition of the precipitate as a function of the amino acid chemistry and concentration. “0” denotes the control sample (no amino acid), which, for simplicity of data representation, was also kept on the log scale of thexaxis. For experimental values, see Table S1.
Figure 4 shows that, in the presence of 1 mM ofL-cysteine, the samples consist of plates and aggregated, parallel rods. At 10 mM, the precipitates form wires. At 100 mM, TEM reveals large platelets with irregular shapes. Some particles show Moire´
patterns or bend contours, demonstrating that they are thin crystalline ﬂakes. TEM therefore again shows that the particle morphology is not controlled by the amino acids. This means that again a wide range of particle sizes and at lowerL-cysteine concentration also a wide range of particle shapes is observed.
Synchrotron XRD of these samples shows a set of sharp reﬂections that can be assigned toL-cystine, that is, the oxidized, dimeric form of L-cysteine. Closer inspection of the XRD patterns also reveals very weak and broad reﬂections at 6.3, 12.2, 16.3, and 21.1 degrees 2θ that can be assigned to the lepidocrocite 200, 210, 301, and 020 reﬂections (JCPDS 44-1415), respectively. XRD thus suggests that here an organic solid containing a small fraction of the inorganic lepidocrocite forms.
Raman spectroscopy, Figure 5, conﬁrms the presence of
L-cystine in the precipitates obtained withL-cysteine as a starting material. Besides the signals assigned toL-cystine, the spectrum also shows a peak at 250 and a shoulder at 377 cm-1, which can be assigned to lepidocrocite.40,41Moreover, X-ray ﬂuores- cence (XRF) shows that the sample contains only ca. 5% of Fe (from lepidocrocite) and ca. 36% of S (fromL-cystine). This is consistent with Raman and XRD data, which also indicate a large amount of organic material. The (molar) organic fraction is 5- to 6-fold larger than the inorganic fraction. Thermogravi- metric analysis (TGA) further conﬁrms these ﬁndings. As a result, Raman, XRF, TGA, and XRD show that the precipitate is an L-cystine/lepidocrocite composite with a high organic fraction.
Amino acid incorporation in the precipitates has been further studied with IR spectroscopy and thermogravimetric analysis (TGA). Figure 6 shows representative TGA curves of a series of samples precipitated withL-lysine. The control sample and samples precipitated from 1 mM solutions only exhibit a minor weight loss, typically less than 0.5%, which is presumably due to water desorption. Samples precipitated withL-threonine and
L-cysteine (with the exception of 100 mML-cysteine, see above)
and all samples precipitated with higher amino acid concentra- tions typically exhibit several broad transitions in TGA (labeled 1, 2, and 3 in Figure 6). The samples lose 3-5% at 70-80°C, followed by an additional loss between 200 and 280 °C, depending on the amino acid (and hence the crystal phases of the original sample). Finally, often a weight loss between 300 and 380°C that again depends on the amino acid is observed.
We assign the ﬁrst weight loss to water leaving the sample.
The two latter losses are assigned to decomposition of the amino acids and iron oxide phase transitions to thermodynamically more stable phases, which is accompanied by dehydration. The width of the transitions however, suggests that the individual processes strongly overlap, and it is therefore difﬁcult to draw more detailed conclusions. XRD however supports this inter- pretation as we only ﬁnd hematite after annealing at 400°C.
This shows that a dehydration and phase transition is involved in the processes observed here.
Figure 7 shows IR spectra of a control sample and a sample precipitated withL-lysine. IR spectroscopy conﬁrms the ﬁndings from TGA and (where applicable) Raman spectroscopy as the samples precipitated with amino acids clearly show the presence of organic moieties in the precipitates. Furthermore, many IR spectra show a signiﬁcant-OH vibration at around 3000-3100 Figure 3. TEM images of (a) control sample (magnetite+goethite),
(b) L-lysine 1 mM (magnetite), (c) L-lysine 10 mM (magnetite + goethite), (d)L-lysine 100 mM (magnetite+goethite+lepidocrocite), (e) L-histidine 60 mM (ferrihydrite), and (f)L-methionine 100 mM (magnetite+lepidocrocite). Scale bars are 100 nm. For fractions of crystal phases see Table 1.
Figure 4. TEM images of precipitates formed in the presence of
L-cysteine. (a, b) 1 mM, (c) 10 mM, and (d) 100 mM. Scale bars are 250 nm. Dark lines (arrows) are bend contours. (e) X-ray pattern of a sample precipitated from a 100 mML-cysteine solution; (x) is a peak from the sample support. Inset: very broad lepidocrocite 200 reﬂection at 6.3 degrees 2θ(arrow).
cm-1. This band is assigned to both water incorporated into the crystal (lattice), in particular in the case of the hydrated iron oxides, and to adsorbed surface water.
The current data provide some basic insight into the effect of single amino acids on the precipitation of iron oxide nanoparticles in vitro. First and foremost, the data show that the different amino acids change the crystal phase of the resulting precipitates. Although the effect is not strong enough to lead to single phase materials, some amino acids have a pronounced effect in that they stabilize large fractions of otherwise unstable crystal phases like ferrihydrite.
Commonly, organic growth modiﬁers are claimed to adsorb onto growing (inorganic) particles, and indeed, an adsorption-
mediated process can also be postulated here. There are two plausible processes that can in principle lead to the observed effects: (1) The amino acids adsorb on the surface of a particle with a given crystal phase as it precipitates. The adsorbed amino acids then prevent redissolution/reprecipitation3of the respective particles. Alternatively, (2) the amino acids adsorb on the surface of the ﬁrst precipitate and then change the redissolution/
reprecipitation process such that different crystal phases form.
Matrajt and Blanot have shown that amino acid adsorption on ferrihydrite differs signiﬁcantly between different amino acids.28 We therefore postulate that in the current study, the amino acids show an amino acid-speciﬁc (or at least partially speciﬁc) adsorption onto particles with different crystal phases. As some amino acids have a higher afﬁnity for metastable phases, they (partly) kinetically trap these phases.
L-Valine and L-methionine have little or no effect on the crystal phase when compared to the control samples. This suggests that there is only a weak interaction (regardless of the type of interaction) between the precipitates and these amino acids. As a result, the crystallization proceeds almost as in the absence of growth modiﬁer.
The other amino acids have signiﬁcant effects on the mineralization. At high concentrations (100 mM), the strongest effects are observed. WithL-arginine,L-lysine, andL-threonine the fractions of metastable crystal phases increase in that order.
That is, these amino acids increasingly stabilize metastable precipitates. Moreover, the metastable crystal phases are stabilized at lower amino acid concentrations than withL-valine and L-methionine. This especially applies to L-threonine and clearly shows that the interaction strength of amino acids and iron oxide particles increases fromL-asparagine toL-threonine.
L-Histidine is somewhat special, because it only affects crystal phase formation at rather high concentration.
The different behavior of the three basic amino acidsL-lysine,
L-arginine, andL-histidine can be rationalized via a rather simple electrostatic interaction model. At pH 9, bothL-lysine (pKaof the residue is 10.28) andL-arginine (pKaof the residue is 13.28) are charged, whereasL-histidine is uncharged (pKaof the residue is 5.97).42As the ferrihydrite surface is positively charged,28,43,44
L-lysine andL-arginine, which also carry positive charges, are repelled from the ferrihydrite surface and therefore show a weaker interaction with the ferrihydrite surface thanL-histidine.
Of the basic amino acids, onlyL-histidine is uncharged and contains donor atoms, which can interact more strongly with the inorganic surface of ferrihydrite.L-Histidine is thus the better stabilizer for the unstable ferrihydrite than the positively charged Figure 5. (a) Raman spectra of L-cysteine, L-cystine, and the
precipitate. (b) Low wavenumber region. Arrows point to lepidocrocite peak and shoulder.
Figure 6. TGA curves of a control sample and samples precipitated with 1, 10, and 100 mM ofL-lysine. Note that theyaxis is only from 50 to 105% relative weight.
Figure 7. Representative IR spectra of a control sample (a) and a sample precipitated with 100 mM ofL-lysine (b). The spectra are drawn to scale and clearly show that some organic components are incorpo- rated into the sample (b).
amino acids. This ﬁnding is supported by earlier experiments,28 where Matrajt and Blanot have shown that L-histidine and
L-threonine adsorb much more efﬁciently on ferrihydrite than the other amino acids used in our study.
Our data support this earlier work, but they also show that uncharged amino acids like L-histidine, L-cysteine, and L- threonine appear to be the better stabilizers for unstable iron oxides. In addition, our study shows that higher amino acid concentrations in some cases stabilize increasingly less stable crystal phases. The most obvious example isL-threonine, where at 1 mM, ca. 50% of the sample are goethite, at 10 mM, the fraction of goethite is lower, but an additional ca. 50% of lepidocrocite form, and at 100 mM only ferrihydrite is observed.
A similar argument can be made forL-cysteine, although there, also, the disulﬁde formation must be taken in account. At lower concentrations there is a diverse group of amino acids, which can trap metastable iron oxide crystal phases, however, usually not as single phase materials.
The above scenario of adsorption and trapping of kinetically favored metastable crystal phases is supported by crystallite size analysis, Table 2. For example, goethite formed in 10 mM solutions ofL-threonine has a coherence length of 47 Å. Goethite precipitated with 10 mM solutions ofL-lysine has a coherence length of 148 Å. This suggests a strong afﬁnity ofL-threonine toward strongly hydrated iron (hydr)oxides, which leads to smaller crystallite size. This further corroborates stabilization via amino acid adsorption and clearly shows that there are large afﬁnity differences between the amino acids and the different crystal phases. TGA and IR further support this ﬁnding by showing evidence for amino acid incorporation into the precipitates.
In summary, our study shows that (1) there are amino acids that are more efﬁcient iron oxide crystal phase modiﬁers than
others and (2) even single amino acids exhibit an incomplete selectivity for certain crystal phases. We suggest that the charges and charge distribution on the different amino acids plays a key role in the mineralization process. Another important parameter for the stabilization of metastable iron oxides is the presence of donor atoms like (uncharged) nitrogen, oxygen, or sulfur atoms. The data suggest that the combination of different amino acids could lead to short peptides that are more speciﬁc crystal phase modiﬁers than individual amino acids. Possibly even mixtures of amino acids could enhance the effects observed here.
Acknowledgment.We thank Dr. M. Neuburger for help with the CSD searches, L. Mirolo for X-ray support, Prof. E. C.
Constable for access to his IR spectrometer, Prof. L. Diamond for access to the Raman spectrometer, and the Swiss National Science Foundation for funding. A.T. thanks the Holcim Stiftung Wissen for a Habilitation Fellowship.
References and Notes
(1) Bauerlein, E.Angew. Chem., Int. Ed.2003,42, 614.
(2) Bauerlein, E.Biomineralization - Progress in Biology, Molecular Biology and Application; Wiley-VCH: Weinheim, Germany, 2004.
(3) Cornell, R. M.; Schwertmann, U. The Iron Oxides: Structure, Properties, Reactions, Occurrences and Uses; Wiley-VCH; Weinheim, Germany, 2003.
(4) Lang, C.; Schu¨ler, D.; Faivre, D.Macromol. Biosci.2007,7, 144.
(5) Gupta, A. K.; Gupta, M.Biomaterials2005,26, 3995.
(6) Tiefenauer, L. X. Magnetic nanoparticles as contrast agents for medical diagnosis. InNanotechnology in Biology and Medicine; Vo-Dinh, T., Ed.; CRC Press LLC: Boca Raton, FL, 2007; pp 29/1.
(7) Douziech-Eryrolles, L.; Marchais, H.; Herve, K.; Munnier, E.;
Souce, M.; Linassier, C.; Dubois, P.; Chourpa, I.Int. J. Nanomed.2007,2, 541.
(8) Lu, A.-H.; Salabas, E. L.; Schu¨th, F.Angew. Chem., Int. Ed.2007, 46, 1222.
(9) Mann, S.; Hannington, J. P.; Williams, R. J. P.Nature1986,324, 565.
(10) Laberty, C.; Navrotsky, A.Geochim. Cosmochim. Acta1998,62, 2905.
(11) Banﬁeld, J. F.; Welch, S. A.; Zhang, H.; Thomsen Ebert, T.; Penn, R. L.Science2000,289, 751.
(12) McGuire, M. M.; Edwards, K. J.; Banﬁeld, J. F.; Hamers, R. J.
Geochim. Cosmochim. Acta2001,65, 1243.
(13) Majzlan, J.; Lang, B. E.; Stevens, R.; Navrotsky, A.; Woodﬁeld, B. F.; Boerio-Goates, J.Am. Mineral.2003,88, 846.
(14) Majzlan, J.; Navrotsky, A.; Schwertmann, U.Geochim. Cosmochim.
(15) Nesterova, M.; Moreau, J.; Banﬁeld, J. F.Geochim. Cosmochim.
(16) Chan, C. S.; De Stasio, G.; Welch, S. A.; Girasole, M.; Frazer, B. H.; Nesterova, M. V.; Fakra, S.; Banﬁeld, J. F.Science2004,303, 1659.
(17) Waychunas, G. A.; Kim, C. S.; Banﬁeld, J. F.J. Nanoparticle Res.
(18) Mazeina, L.; Deore, S.; Navrotsky, A.Chem. Mater.2006,18, 1830.
(19) Mazeina, L.; Navrotsky, A.Clays Clay Minerals2005,53, 113.
(20) Matsunaga, T.; Suzuki, T.; Tanaka, M.; Arakaki, A. Trends Biotechnol.2007,25, 182.
(21) Staniland, S.; Ward, B.; Harrison, A.; van der Laan, G.; Telling, N.Proc. Natl. Acad. Sci. USA2007,104, 19524.
(22) Faivre, D.; Bo¨ttger, L. H.; Matzanke, B. F.; Schu¨ler, D.Angew.
Chem., Int. Ed.2007,46, 8495.
(23) Navrotsky, A.; Mazeina, L.; Majzlan, J.Science2008,319, 1635.
(24) Brown, S.Proc. Natl. Acad. Sci. U.S.A.1992,89, 8651.
(25) Brown, S.; Sarikaya, M.; Johnson, E.J. Mol. Biol.2000,299, 725.
(26) Arakaki, A.; Webb, J.; Matsunaga, T.J. Biol. Chem.2003,278, 8745.
(27) Prozorow, T.; Mallapragada, S. K.; Narasimhan, B.; Wang, L.; Palo, P.; Nilsen-Hamilton, M.; Wiiliams, T. J.; Bazylinski, D. A.; Prozorow, R.;
Canﬁeld, P.AdV. Funct. Mater.2007,17, 951.
(28) Matrajt, G.; Blanot, D.Amino Acids2004,26, 153.
TABLE 2: Size (Anisotropy) of the Particles Analysis of the Samples Determined from Rietveld Reﬁnementa
1 mM 10 mM 100 mMb
control sample mag: 566.06 (0.36)
goe: 64.47 (0.15)
L-valine mag: 209.27 (0.15) mag: 123.89 (0.08) mag: 27.07 (0.02) goe: n/ac lep: 84.48 (0.06)
L-lysine mag:172.56 (0.11) mag: 148.49 (0.3) mag: 27.07 (0.02) goe: 148.39 (0.3) goe: n/ac
lep: 84.48 (0.12)
L-methionine mag: 291 mag: 62 mag: 30
goe: 62.24 lep: 44.59
L-asparagine mag: 175.13 (0.13) mag: 62.97 (0.08) mag: 55.42 (0.06)
goe: 24.73 (0.04) goe: 46.61 (0.10)
lep: 69.10 (0.10)
L-arginine mag: 255.24 (0.04) mag: 65.46 (0.06) mag: 53.01 (0.05) goe: 126.66 (0.34) goe: 35.66 (0.06)
lep: 69.08 (0.07)
L-histidine mag: 294.24 (0.02) mag: 104.50 (0.09) fer: n/ac
L-threonine mag: 95.13 (0.13) mag: 44.04 (0.2) fer: n/ac goe: 13.95 (0.01) goe: 47.08 (0.03)
lep: 80.27 (0.13)
L-cysteine mag: 231.69 (0.17) lep: 52.11 (0.06) n/ac goe: 113.37 (0.16)
lep: 305.44 (0.31)
aMag: magnetite, Goe: goethite, Lep: lepidocrocite, Fer:
ferrihydrite, n/a: not applicable due to too low peak intensity or too broad reﬂections. Sizes are given in Å. bMaximum concentrations are 80 mM for L-threonine and 60 mM for L-histidine. cSome values could not be determined due to too broad lines, where Rietveld reﬁnement was not successful.
(29) Sarikaya, M.; Tamerler, C.; Jen, A. K. Y.; Schulten, K.; Baneyx, F.Nat. Mater.2003,2, 577.
(30) Gerstel, P.; Hoffmann, R. C.; Lipowsky, P.; Jeurgens, L. P. H.;
Bill, J.; Aldinger, F.Chem. Mater.2006,18, 179.
(31) Bauermann, L. P.; Bill, J.; Aldinger, F. J. Phys. Chem B2006, 110, 5182.
(32) Taubert, A.; Palms, D.; Glasser, G.Langmuir2002,18, 4488.
(33) Taubert, A.; Palms, D.; Weiss, O¨ .; Piccini, M.-T.; Batchelder, D. N.
Chem. Mater.2002,14, 2594.
(34) Taubert, A.; Ku¨bel, C.; Martin, D. C.J. Phys. Chem B2003,107, 2660.
(35) Rao, P. V.; Holm, R. H.Chem. ReV.2004,104, 527.
(36) Schmitt, B.; Bro¨nnimann, C.; Eikenberrya, E. F.; Gozzo, F.;
Ho¨rmann, C.; Horisberger, C.; Patterson, B.Nuclear Instrum Methods Phys Res A2003,501, 267.
(37) http://www-llb.cea.fr/fullweb/fp2k/fp2k.htm, August, 2006.
(38) Oner, M.; Norwig, J.; Meyer, W. H.; Wegner, G.Chem. Mater.
(39) Wegner, G.; Baum, P.; Muller, M.; Norwig, J.; Landfester, K.
Macromol. Symp.2001,175, 349.
(40) Nobuyuki, T.; Kolthoff, I. M.; Stricks, W.J. Am. Chem. Soc.1955, 77, 1996.
(41) Chang, S.-G.; Littlejohn, D.; Liu, D. K.Ind. Eng. Chem. Res.1988, 27, 2156.
(42) Windholz, M.; Budavari, S.; Stecher, P. G.The Merck Index, 8th ed.; Merck: Rahway, NJ, 1968.
(43) Charlet, L.; Manceau, A. A.J. Colloid Interface Sci.1992,148, 425.
(44) Davis, J. A.; Leckie, J. O.J. Colloid Interface Sci.1978,67, 90.